Enhanced proton conduction by post-synthetic covalent modification in a porous covalent framework
Samanta, Partha; Desai, Aamod V.; Anothumakkool, Bihag; Shirolkar, Mandar M.; Karmakar, Avishek; Kurungot, Sreekumar; Ghosh, Sujit K.; Journal of Materials Chemistry A 5 (2017) 13659–; doi:10.1039/C7TA00964J

data_7236543
_publ_section_title
;
 Enhanced proton conduction by post-synthetic covalent modification in a
 porous covalent framework
;
_journal_issue                   26
_journal_name_full               'Journal of Materials Chemistry A'
_journal_page_first              13659
_journal_paper_doi               10.1039/C7TA00964J
_journal_volume                  5
_journal_year                    2017
_chemical_formula_moiety         'C42 H33 N3 O6'
_chemical_formula_sum            'C42 H33 N3 O6'
_chemical_formula_weight         675.71
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-11-04 deposited with the CCDC.
2017-05-30 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 118.439(3)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   26.787(4)
_cell_length_b                   15.382(2)
_cell_length_c                   20.723(3)
_cell_measurement_temperature    150(2)
_cell_volume                     7508.3(19)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.990
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0578
_diffrn_reflns_av_unetI/netI     0.0474
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_limit_h_max       35
_diffrn_reflns_limit_h_min       -35
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            65003
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.484
_diffrn_reflns_theta_min         1.581
_exptl_absorpt_coefficient_mu    0.081
_exptl_crystal_colour            'Light yellow'
_exptl_crystal_density_diffrn    1.196
_exptl_crystal_description       Needle
_exptl_crystal_F_000             2832
_platon_squeeze_details
;
;
_refine_diff_density_max         0.847
_refine_diff_density_min         -0.831
_refine_diff_density_rms         0.110
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.958
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     451
_refine_ls_number_reflns         9409
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      0.964
_refine_ls_R_factor_all          0.1509
_refine_ls_R_factor_gt           0.1250
_refine_ls_shift/su_max          0.023
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1495P)^2^+71.9047P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3296
_refine_ls_wR_factor_ref         0.3445
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6562
_reflns_number_total             9409
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7ta00964j2.cif
_cod_data_source_block           Squeezed
_cod_original_cell_volume        7507.8(18)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7236543
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              89795
_shelx_hkl_checksum              38568